Polymorphic transformations in glycine co-crystals at low temperature and high pressure: two new examples as a follow-up to a glycine‒glutaric acid study
Losev, E. A.; Zakharov, B. A.; Boldyreva, E. V.; CrystEngComm 18 (2016) 5869–; doi:10.1039/C6CE00561F

data_7225635
_publ_section_title
;
 Polymorphic transformations in glycine co-crystals at low temperature and
 high pressure: two new examples as a follow-up to a glycine--glutaric
 acid study
;
_journal_issue                   31
_journal_name_full               CrystEngComm
_journal_page_first              5869
_journal_paper_doi               10.1039/C6CE00561F
_journal_volume                  18
_journal_year                    2016
_chemical_formula_moiety         'C4 H6 O6, C2 H5 N O2'
_chemical_formula_sum            'C6 H11 N O8'
_chemical_formula_weight         225.16
_chemical_name_common            'glycine-DL-tartaric acid (1:1)'
_chemical_name_systematic        'glycine-DL-tartaric acid (1:1)'
_space_group_crystal_system      triclinic
_space_group_IT_number           2
_space_group_name_Hall           '-P 1'
_space_group_name_H-M_alt        'P -1'
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-2014/7
_audit_update_record
;
2016-06-16 deposited with the CCDC.
2016-06-20 downloaded from the CCDC.
;
_cell_angle_alpha                99.633(7)
_cell_angle_beta                 95.811(5)
_cell_angle_gamma                94.695(6)
_cell_formula_units_Z            4
_cell_length_a                   4.7136(3)
_cell_length_b                   8.9774(10)
_cell_length_c                   18.3305(11)
_cell_measurement_pressure       3570000
_cell_measurement_reflns_used    1158
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      28.0726
_cell_measurement_theta_min      2.2695
_cell_volume                     756.94(11)
_computing_cell_refinement
;
CrysAlisPro, Agilent Technologies,
Version 1.171.35.21 (release 20-01-2012 CrysAlis171 .NET)
(compiled Jan 23 2012,18:06:46)
;
_computing_data_collection
;
CrysAlisPro, Agilent Technologies,
Version 1.171.35.21 (release 20-01-2012 CrysAlis171 .NET)
(compiled Jan 23 2012,18:06:46)
;
_computing_data_reduction
;
CrysAlisPro, Agilent Technologies,
Version 1.171.35.21 (release 20-01-2012 CrysAlis171 .NET)
(compiled Jan 23 2012,18:06:46)
;
_computing_molecular_graphics    'Mercury (Macrae et al., 2006)'
_computing_publication_material
;
Mercury (Macrae et al., 2006), 
PLATON (Spek, 2009),
;
_computing_structure_refinement  'SHELXL-2014/7 (Sheldrick, 2014)'
_computing_structure_solution    'SIR2014 Version 14.10 (Burla, 2015)'
_diffrn_ambient_pressure         3570000
_diffrn_ambient_temperature      293(2)
_diffrn_detector_area_resol_mean 10.3457
_diffrn_measured_fraction_theta_full 0.350
_diffrn_measured_fraction_theta_max 0.301
_diffrn_measurement_device_type  'Xcalibur, Ruby, Gemini'
_diffrn_measurement_method       \w-scan
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.1274
_diffrn_reflns_av_unetI/netI     0.1099
_diffrn_reflns_Laue_measured_fraction_full 0.350
_diffrn_reflns_Laue_measured_fraction_max 0.301
_diffrn_reflns_limit_h_max       6
_diffrn_reflns_limit_h_min       -6
_diffrn_reflns_limit_k_max       7
_diffrn_reflns_limit_k_min       -7
_diffrn_reflns_limit_l_max       23
_diffrn_reflns_limit_l_min       -23
_diffrn_reflns_number            4161
_diffrn_reflns_point_group_measured_fraction_full 0.350
_diffrn_reflns_point_group_measured_fraction_max 0.301
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         28.072
_diffrn_reflns_theta_min         2.269
_diffrn_source                   'Enhance (Mo) X-ray Source'
_exptl_absorpt_coefficient_mu    0.188
_exptl_absorpt_correction_T_max  0.480
_exptl_absorpt_correction_T_min  0.395
_exptl_absorpt_correction_type   gaussian
_exptl_absorpt_process_details   'Absorb-7 (Angel, 2013)'
_exptl_crystal_colour            colourless
_exptl_crystal_density_diffrn    1.976
_exptl_crystal_description       block
_exptl_crystal_F_000             472
_exptl_crystal_size_max          0.160
_exptl_crystal_size_mid          0.060
_exptl_crystal_size_min          0.030
_refine_diff_density_max         0.432
_refine_diff_density_min         -0.427
_refine_diff_density_rms         0.084
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.083
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     121
_refine_ls_number_reflns         1105
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.083
_refine_ls_R_factor_all          0.1464
_refine_ls_R_factor_gt           0.0943
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.1536P)^2^+0.7060P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.2387
_refine_ls_wR_factor_ref         0.2875
_reflns_Friedel_coverage         0.000
_reflns_number_gt                665
_reflns_number_total             1105
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            c6ce00561f17.cif
_cod_data_source_block           gta357GPa
_cod_depositor_comments
;
The following automatic conversions were performed:

'_exptl_absorpt_correction_type' value 'Gaussian' changed to
'gaussian' according to
/usr/data/users/saulius/crontab/automatic-downloads/rss-feeds/RSC/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 4268 2015-11-12 08:31:59Z antanas 

 Adding full bibliography for 7225609--7225638.cif.
;
_cod_original_cell_volume        756.93(11)
_cod_database_code               7225635
_shelx_shelxl_version_number     2014/7
_shelx_estimated_absorpt_t_min   0.971
_shelx_estimated_absorpt_t_max   0.994
_shelx_res_checksum              73568